2Definition:When materials under severe service conditions are required to sustain steady loads for long periods of time, they undergoa time dependent deformation.This is known as creep
3CREEPcan also be defined as‘ the slow and progressive deformation of a material with time at constant stress.’
4Creep is found to occur at higher temperature than at lower temp. Therefore the study of creep is very important for those materials which are used at high temp like components of gas turbines, furnaces, rockets, missiles etc.
5Creep curve:The creep curve is obtained by applying a constant tensile load below the yield point to a specimen maintained at constant temp.
11Primary creep: OR TRANSIENT CREEP This is the first stage of the creep which represents a region of decreasing creep rate.
12In this region the rate at which the material deforms decreases with time until it reaches a constant value.
13The creep rate goes on reducing because as the metal deforms it undergoes strain hardening and offers more and more resistance to further elongation.
14Transient creep:The principle characteristic of transient creep is the decreasing rate in deformation.Deformation is rapid at first but gradually becomes slower and slower as the rate approaches some fixed value.Transient creep in metals is observed at all temp, even near absolute zero. Hence it is some times referred to as ‘cold creep’
15Nearly constant creep rate, Secondary creep: [steady state creep]Nearly constant creep rate,because strain-hardening and recovery effectsbalance each other.Creep in this region takes place by the viscous flow in the materials.
16Viscous creep: SECONDARY CREEP] It is characterized by the viscous flow of the material means that there is a constant or a steady increase in deformation at constant stress.
17Although strain hardening is present, its effect is just balanced by the ‘recovery’ process which has the opposite effecti.e softening the metal.
18viscous creep is stopped when there is considerable reduction in cross sectional area and enters the tertiary stage .The rate of deformation increases rapidly in this 3rd stage and fracture occurs at the end of this stage.
19Viscous creep also known as ‘hot creep', since it is observed only at higher temperature.
20Tertiary creep :This stage is period of increasing strain rate.Tertiary creep occurs when there is an effective reduction in cross-sectional area due to necking or internal void formation.
21then the resulting fracture due to creep would be at ‘B’. If the stress is kept constant of the load or if true strain is taken into considerationthen the resulting fracture due to creep would be at ‘B’.
22lower temp have an effect of decreasing the creep rate. Effect of low temperature :Temperature below Tm/4 are called as LOWER TEMP.lower temp have an effect of decreasing the creep rate.This is because strain hardening effects will be more and recovery process is negligible.
24ε = α ln t where ε - strain , α – a constant t – time . Creep occurring at lower temp is known as ‘logarithmic creep’ε = α ln twhere ε - strain ,α – a constantt – time .
25low temp. logarithmic creep obeys a mechanical equation of state i low temp. logarithmic creep obeys a mechanical equation of state i.e the rate of strain at a given time depends only on the instantaneous values of stress and strain and not on the previous strain history.
26Effect of high temperature: At Higher temp. the creep rate increases.‘ structural changes’ takes place.
27Mobility of atoms increases with temp and occupy lower energy positions.Mobility of dislocation also increases and they overcome the obstacles by the mechanism of climb.
28The concentration of vacancies increases with temp and the rate of diffusion increases.Recrystallization takes place as a result of increased rate of diffusion.
29Grains in polycrystalline materials move relative to each other . This grain- boundary sliding is a shear process which occurs in the direction of the grain boundary and leads to intergranular cracks.
30Dislocation creep or dislocation climb Diffusion creep Mechanism of creep: The chief mechanism responsible for creep deformation are ,Dislocation glideDislocation creep or dislocation climbDiffusion creepGrain boundary sliding.
311) Dislocation glide :The creep rate is established by the ease with which the dislocation move across obstacles such as precipitates, GB etc.
33This may include cross-slip of dislocations with the aid of thermal energy. Dislocation glide results in increase in plastic strain during creep deformation
34This is caused due to mutual movement of dislocations & vacancies. 2) Dislocation creep or dislocation climb:This is caused due to mutual movement of dislocations & vacancies.
35This is called dislocation climb. At high temp the diffusion rate of vacancies is more which make the dislocations to glide & climb,edge dislocation can move end of a slip planeOR to a plane above or below the slip Plane.This is called dislocation climb.
36.DislocationVacancyMutual movement ofdislocations & vacancies.
37This occurs at high temperature (T>0.4Tm) &When dislocation cause across obstacles,they use vacancies/or interstitial atoms to climb and go around them for slip &hence plastic deformation continues.
38It occurs when temp. is high & at relatively low stresses. 3) Diffusion creep: -It occurs when temp. is high & at relatively low stresses.diffusion of vacancies controls the creep rate.But edge dislocation is not involved in them.
39vacancies move from the surface of the specimen towards the stress axis
40i.e when load is applied & kept constant ,the vertical boundaries are subjected to compression & the horizontal grain boundaries are subjected to tensile stress.
41so vacancies migrate from tensile region to compression region & atoms migrate in opposite direction to vacancies.i.e causing the creep strain along tensile axis,
42the mechanism is called Nabarro-herring creep because the flux of atoms is through the bulk of atoms.
434) Grain boundary sliding:- At low temp the Grain boundaries will not flow viscously & provide obstacles to dislocation motion.
44At elevated temp , the grains in polycrystalline materials are able to move relative to each other, this is called grain boundary sliding and is an shear process which occurs in the direction of grain boundary [GB] .
45a large no. of grains sliding with each other results in plastic deformation due to creep . GB sliding is promoted by increases the temp. T & or decreasing the strain rate.
46In fine grained materials because of large no In fine grained materials because of large no. of grains this type of creep is more ,so to avoid it large-coarse grained materials are to be used.
47Ex :Ni-based super alloy with single crystals in jet engine blades, eliminates the possibility of creep at high temp aided by grain boundary sliding
48Stress relaxation :-Stress relaxation is the time dependent decrease in stress acting on a body which is constrained to a certain fixed deformation.In other words it is the reduction in the value of stress in those compounds which are not allowed to elongate.
49Ex :stress relaxation in bolts which hold rigid bodies in tight contact , stress will reduce in such numbers after a long period.
50Expression for stress relaxation : Consider a tensile specimen which is subjected to a constant initial stress σi at elevated temp.The total strain of the specimen is givenε = εe+ εPThis eqn. is the expression for stress relaxation this gives the value of stress ( σ) at any instant of time t with initial stress being σi.It is seen form the relation that (σ α 1/t)i.e σ is inversely propotional to it.i.e stress σ goes on decreasing with time with other quantities being constant temp ,T1,T2,T , T1< T2< T3.Fig stress relaxation curves.
53Creep properties :-1) creep strength/ or creep limit:It is defined as the highest stress that material can withstand without excessive deformation for a specified length of time.
54Ex :- creep strength for a steam turbine blade may be that stress which will produce just 0.2% creep for 10,000 hours of working at 800oC.
55Creep strength can also be defined as the stress at given temperature which produces steady state creep rate of fixed amount say to /sec.ORIt is the stress to cause a creep strain of 1% in fixed time say 105 hours.
562) Creep rupture strength:- it is defined as the highest stress that a material can withstand without rupture for a specified length of time.Ex : For the same turbine blade . the rupture strength is that stress which produces a fracture in 1000HR OR 10000HR OR hrs at 800oC.
57Thus creep rupture strength is also defined as the limiting stress below which creep is so slow that will not result in fracture within any finite length of time.It is also called as” stress ruptures strength”.
58TIME to fracture under a given static load. 3) Creep life:it is defined as theTIME to fracture under a given static load.C
60Load : Creep rate increases as load increases. Temperature: Creep rate increases as T increases.Composition: Pure metals are softer than alloys , the different phases present stops the dislocation glide .Hence creep is more in pure metals.
61Grain size: “Smaller the grain, stronger the material.” But above Equicohessive temp. this effect will be reversed one.Equicohessive temp. (Kelvin) Te > Tm/2Heat Treatment: This changes the structure,Obviously the materials property changes, creep resistance also changes.